DOI: 10.1038/ncomms3265

Quantum criticality in electron-doped BaFe2 xNixAs2 R. Zhou1, Z. Li1, J. Yang1, D.L. Sun2, C.T. Lin2 & Guo-qing Zheng1,3

A quantum critical point is a point in a system’s phase diagram at which an order is completely suppressed at absolute zero temperature (T). The presence of a quantum critical point manifests itself in the ﬁnite-T physical properties, and often gives rise to new states of matter. Superconductivity in the cuprates and in heavy fermion materials is believed by many to be mediated by ﬂuctuations associated with a quantum critical point. In the recently discovered iron–pnictide superconductors, we report transport and NMR measurements on BaFe2 xNixAs2 (0rxr0.17). We ﬁnd two critical points at xc1 ¼ 0.10 and xc2 ¼ 0.14. The electrical resistivity follows r ¼ r0 þ ATn, with n ¼ 1 around xc1 and another minimal n ¼ 1.1 at xc2. By NMR measurements, we identity xc1 to be a magnetic quantum critical point and suggest that xc2 is a new type of quantum critical point associated with a nematic structural phase transition. Our results suggest that the superconductivity in carrier-doped pnictides is closely linked to the quantum criticality.

1 Beijing National Laboratory for Condensed Matter Physics, Institute of Physics, Chinese Academy of Sciences, Beijing 100190, China. 2 Max Planck InstituteHeisenbergstrasse 1, D-70569 Stuttgart, Germany. 3 Department of Physics, Okayama University, Okayama 700-8530, Japan. Correspondence and requests for materials should be addressed to G.-q.Z. (email: [email protected]).

NATURE COMMUNICATIONS | 4:2265 | DOI: 10.1038/ncomms3265 | www.nature.com/naturecommunications

& 2013 Macmillan Publishers Limited. All rights reserved.

1

ARTICLE

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms3265

Results Electrical resistivity measurements. Figure 1 shows the in-plane electrical resistivity data in BaFe2 xNixAs2 for various x, which are ﬁtted by the equation rab ¼ r0 þ ATn (for data over the whole

4 3

0.15

2 1

0.1

0 150

BaFe2–xNixAs2 2

100

n 1

50

AF

AF+SC

0

–50 0.00

0.05

0.10

0.15

0.20

x Figure 2 | The obtained phase diagram of BaFe2 xNixAs2. (a) The residual resistivity r0 and the coefﬁcient A as a function of Ni-doping x. (b) The obtained phase diagram of BaFe2 xNixAs2. The TN and y are obtained from NMR spectra and 1/T1T, respectively. AF and SC denote the antiferromagnetically ordered and the superconducting states, respectively. The solid and dashed lines are the guides to the eyes. Colours in the normal state represent the evolution of the exponent n in the resistivity ﬁtted by rab ¼ r0 þ ATn. The light yellow region at x ¼ 0.10 shows that the resistivity is T-linear. The error bar for y is the s.d. in the ﬁtting of 1/T1T. The error bar for Ts represents the temperature interval in measuring the NMR spectra.

BaFe2–x Nix As2

BaFe2–x Nix As2 ~ T 1.1

x=0

~ T 1.6

SC

Tc TN Ts θ

2.5

2

A (10–4 mΩ cm K–n)

5

0.2 0 (mΩ cm)

I

temperature range, see Supplementary Fig. S1 and Supplementary Note 1). For a conventional metal described by the Fermi liquid theory, the exponent n ¼ 2 is expected. However, we ﬁnd no1.5

Temperature (K)

n cuprate high temperature superconductors1 and heavy fermion2 compounds, the superconductivity is accompanied by the normal-state properties deviated from a Landau–Fermi liquid. Such deviation has been ascribed to the quantum critical ﬂuctuations associated with a quantum critical point (QCP)3,4, whose relationship to the occurrence of superconductivity has been one of the central issues in condensed-matter physics in the last decades. In iron–pnictide high-temperature superconductors5,6, searching for magnetic ﬂuctuations has also become an important subject7. Quantum critical ﬂuctuations of order parameters take place not only in spatial domain, but also in imaginary time domain8,9. The correlation time t0 and correlation length x are scaled to each other, through a dynamical exponent z, t0pxz. Several physical quantities, such as the electrical resistivity and spinlattice relaxation rate (1/T1), can be used to probe the quantum critical phenomena. For the quasiparticles scattering dominated by the quantum critical ﬂuctuations, the resistivity scales as rpTn. For a two-dimensional (2D) antiferromagnetic spin-density wave (SDW) QCP, the exponent n ¼ 1 is often observed1,2,10. On the other hand, for a 2D order with q ¼ (0,0) where z ¼ 3, n ¼ 4/3 at the QCP11,12. Around a QCP, 1/T1 also shows a characteristic T-scaling11. BaFe2 xNixAs2 is an electron-doped system13 where every Ni donates two electrons in contrast to Co doping that contributes only one electron14. Therefore, Ni doping suffers less from disorder which is usually harmful for a QCP to exist. In this work, we ﬁnd two critical points at xc1 ¼ 0.10 and xc2 ¼ 0.14, respectively. By NMR measurements, we identify xc1 to be a magnetic QCP and suggest that xc2 is a QCP associated with the tetragonal-to-orthorhombic structural phase transition. The highest Tc is found around xc1, which suggests that the superconductivity in the carrier-doped BaFe2As2 is more closely tied to the magnetic QCP, while the unusual quantum criticality associated with the structural transition deserves further investigation.

x = 0.14

x = 0.10

0.2

ab (mΩ cm)

ab (mΩ cm)

~ T 1.0 1.5

1

x = 0.12 ~ T 1.3

x = 0.07 ~ T 1.6

x = 0.09 ~ T 1.45

0.5 ~ T 1.8

x = 0.05 x = 0.17 ~ T 1.7

0

0.1 50

100

150

Temperature (K)

200

0

50

100

Temperature (K)

Figure 1 | The in-plane electrical resistivity. The in-plane electrical resistivity rab for BaFe2 xNixAs2. The data in the normal state are ﬁtted by the equation rab ¼ r0 þ ATn (red curve). 2

NATURE COMMUNICATIONS | 4:2265 | DOI: 10.1038/ncomms3265 | www.nature.com/naturecommunications

& 2013 Macmillan Publishers Limited. All rights reserved.

ARTICLE

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms3265

for 0.09rxr0.14. This is a notable feature of non-Fermi liquid behaviour. Most remarkably, a T-linear behaviour (n ¼ 1) is observed for xc1 ¼ 0.10 and persists up to T ¼ 100 K. Another minimal n ¼ 1.1 is found for xc2 ¼ 0.14, which is in good agreement with a previous transport measurement15. An equally interesting feature is that both the residual resistivity r0 and the coefﬁcient A show a maximum at xc1 and xc2 as seen in Fig. 2a. The evolution of the exponent n with Ni content is shown in Fig. 2b.

T= 100 K

H0 = 11.998 T

102 T= 15 K

BaFe1.93Ni0.07As2 75

As-NMR

T= 50 K

BaFe1.93Ni0.07As2 H0 c

TN

101

H0 = 11.998 T T= 25 K

75

80 85 90 95 Frequency (MHz)

100

Tc ~T

100 ~T 3

BaFe1.90Ni0.10As2 H0 c H0 = 11.998 T

intensity (a.u.)

75As-NMR

BaFe1.95Ni0.05As2 H0 c

1/T1 (s–1)

75As-NMR intensity (a.u.)

75As-NMR intensity (a.u.)

NMR measurements. We use NMR to investigate the nature of xc1 and xc2. We identify xc1 to be a SDW QCP and suggest that xc2 is a tetragonal-to-orthorhombic structural phase transition QCP. Figure 3a,b display the frequency-swept spectra of 75As NMR for x ¼ 0.05 and 0.07, respectively. The very narrow central transition peak above the antiferromagnetic transition temperature TN testiﬁes a good quality of the samples. When a magnetic order sets in, the spectra will split into two pairs as labelled in Fig. 3a, due to the development of an internal magnetic ﬁeld Hint. For x ¼ 0.05, we observed two split broad peaks below TN ¼ 74 K. This is due to a distribution of Hint, which results in a broadening of each pair of the peaks. Upon further doping, Hint is reduced and its distribution becomes larger, so that only one broad peak can be seen below TN ¼ 48 K for x ¼ 0.07. Similar broadening of the spectra was also observed previously in a very lightly-doped sample BaFe1.934Ni0.066As2 (ref. 16). For both x, the spectra can be reproduced by assuming a Gaussian distribution of Hint as shown

by the red curves. We obtain the averaged internal ﬁeld /HintS ¼ 0.75 T at T ¼ 15 K for x ¼ 0.05, and /HintS ¼ 0.39 T at T ¼ 25 K for x ¼ 0.07. By using a hyperﬁne coupling constant of 1.88 T per mB obtained in the undoped parent compound17, the averaged ordered magnetic moment /SS is deduced. As seen in Fig. 4, the ordered magnetic moment develops continuously below TN, being consistent with the second-order nature of the phase transition. It saturates to 0.43 mB for x ¼ 0.05, and 0.24 mB for x ¼ 0.07, respectively. The ordered moment is smaller than that in the hole-doped Ba1 xKxFe2As2 (ref. 18), which is probably due to the fact that Ni goes directly into the Fe site and is more effective in suppressing the magnetic order. Upon further doping, at x ¼ 0.09 and x ¼ 0.10, however, no antiferromagnetic transition was found, as demonstrated in Fig. 3c, which shows no splitting or broadening ascribable to a magnetic ordering. The onset of the magnetic order in the underdoped regime is also clearly seen in the spin-lattice relaxation. Figure 3d shows 1/T1 for x ¼ 0.07, which was measured at the position indicated by the arrow in Fig. 3b, in order to avoid any inﬂuence from possible remnant paramagnetic phase, if any. As seen in Fig. 3d, a clear peak is found at TN ¼ 48 K due to a critical slowing down of the magnetic moments. Below TN, 1/T1 decreases down to Tc. Most remarkably, 1/T1 shows a further rapid decrease below Tc, exhibiting a T3 behaviour down to T ¼ 5 K. Such a signiﬁcant decrease of 1/T1 just below Tc is due to the superconducting gap opening in the antiferromagnetically ordered state. This is clear and direct evidence for a microscopic coexistence of

15.9 K 1.89 K

10–1

87.6

87.7

101

102 Temperature (K)

87.8

Frequency (MHz) Figure 3 | NMR spectra with doping and temperature dependence of 1/T1 at optimal doping. 75As-NMR spectra obtained by sweeping the frequency at a ﬁxed external ﬁeld H0 ¼ 11.998 T applied along the c axis. (a) The spectra above and below TN ¼ 74 K for x ¼ 0.05. Solid, dashed and dotted lines indicate, respectively, the position of the central transition, left- and right-satellites, when an internal magnetic ﬁeld develops. (b) The spectra above and below TN ¼ 48 K for x ¼ 0.07. The red curve represents the simulations by assuming a Gaussian distribution of the internal magnetic ﬁeld. The black arrow indicates the position at which T1 is measured below TN. (c) The central transition line at and below Tc for x ¼ 0.10. The spectrum shift at T ¼ 1.89 K is due to a reduction of the Knight shift in the superconducting state. (d) The temperature dependence of 1/T1 for x ¼ 0.07. The solid and dashed lines show the T3- and T-variation, respectively. The solid and dashed arrows indicate Tc and TN, respectively. The error bar in 1/T1 is the s.d. in ﬁtting the nuclear magnetization recovery curve. NATURE COMMUNICATIONS | 4:2265 | DOI: 10.1038/ncomms3265 | www.nature.com/naturecommunications

& 2013 Macmillan Publishers Limited. All rights reserved.

3

ARTICLE

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms3265

0.6 Tc

0.5

BaFe1.93Ni0.07As2

1.2

BaFe2–xNixAs2

0.3

(T)

0.3 0.2

0.1

0.1 0

(B)

0.2

1/T1T (s–1 K–1)

1.0 0.4

TN 0

10

20

30

40

50

0.6 0.4 0.2

0 60

0.0 0

Temperature (K)

intra

seen in Ba(Fe1 xCox)2As2 (ref. 19). We analyse the (1/T1T)AF part by the self-consistent renormalization theory for a 2D itinerant electron system near a QCP11, which predicts that 1/T1T is proportional to the staggered magnetic susceptibility w00 (Q). As w00 (Q) follows a Curie–Weiss law11, one has T11T ¼ T þa y. The AF

intraband contribution is due to the density of state at the Fermi level, which is related to the spin Knight shift (Ks) through the Korringa relation Ks2 T1 T ¼ constant20. The Knight shift was found to follow a T-dependence of K ¼ K0 þ Ksexp( Eg/kBT) as seen in Fig. 5b, where K0 is T-independent, while the second is due to the band that sinks below the Fermi 21,22 level . Correspondingly, we can write T11T ¼ b þ c intra exp 2Eg =kB T . The resulting y is plotted in Fig. 2b. Note that y is almost zero at x ¼ 0.10, which yields a constant 1/T1 above Tc as seen in Fig. 6. The result of y ¼ 0 means that the staggered magnetic susceptibility diverges at T ¼ 0, indicating that x ¼ 0.10 is a magnetic QCP. Therefore, the exponent n ¼ 1 in the resistivity is due to the magnetic QCP (Generally speaking, scatterings due to the magnetic hot spots give a T-linear resistivity11, but those by other parts of the Fermi surface will not23,24. In real materials, however, there always exist some extent of impurity scatterings that can connect the magnetic hot spots 4

200

300

0.32 BaFe2–xNixAs2 0.30

K (%)

superconductivity and antiferromagnetism, as the nuclei being measured experience an internal magnetic ﬁeld yet the relaxation rate is suppressed rapidly below Tc. For x ¼ 0.10, as mentioned already, no antiferromagnetic transition was found. Namely TN ¼ 0. This is consistent with the extrapolation of the TN versus x relation that gives a critical point that coincides with xc1 ¼ 0.10, which is further supported by the spin dynamics as elaborated below. Figure 5a shows the quantity 1/T1T for 0.05rxr0.14. The 1/T1T decreases with increasing T down to around 150 K, but starts to increase towards TN or Tc. The increase T is due to at low 1 the antiferromagnetic spin ﬂuctuation T1 T AF , and the 1 decrease at high T is due to an intraband effect T1 T intra . Namely, T11 T ¼ T11T þ T11T . A similar behaviour was also

100

Temperature (K)

Figure 4 | The temperature dependence of the internal magnetic ﬁeld and the ordered moment for x ¼ 0.07. Temperature dependence of the averaged internal magnetic ﬁeld /HintS (left vertical axis) and the averaged ordered moment /SS (right vertical axis) for x ¼ 0.07. The solid and dashed arrows indicate Tc and TN, respectively. The error bar represents the absolute maxima (minima) that can ﬁt a spectrum.

AF

x = 0.05 x = 0.07 x = 0.09 x = 0.10 x = 0.12 x = 0.14

0.8

0.28 x = 0.05 x = 0.07 x = 0.09 x = 0.10 x = 0.12 x = 0.14

0.26 0.24 0.22

0

100

200

300

Temperature (K) Figure 5 | The quantity 1/T1T and the Knight shift. (a) Temperature dependence of 1/T1T and (b) the Knight shift K for various x. The solid line is a ﬁtting of T11T ¼ T þa y þ b þ c expð 2Eg =kB T Þ. The dashed curve is a ﬁt to K ¼ K0 þ Ks exp( Eg /kBT). The obtained parameters are Eg /kB ¼ 620±40, 510±40, 370±30, 365±30, 350±30 and 330±30 K for x ¼ 0.05, 0.07, 0.09, 0.10, 0.12 and 0.14, respectively. The solid and dashed arrows indicate Tc and TN, respectively. The error bar for 1/T1T is the s.d. in ﬁtting the nuclear magnetization recovery curve. The error bar for K was estimated by assuming that the spectrum-peak uncertainty equals the point (frequency) interval in measuring the NMR spectra.

and other parts of the Fermi surface as to restore the n ¼ 1 behaviour at a magnetic QCP). Next, we use 75As NMR to study the structural phase transition. A tetragonal-to-orthorhombic structural transition was found in the parent compound25, but no direct evidence for such structural transition was obtained in the doped BaFe2 xNixAs2 thus far. In BaFe2 xCoxAs2, a structural transition was detected in the low-doping region26, but it is unclear how the transition temperature Ts would evolve as doping level increases. The 75As nucleus has a nuclear quadrupole moment that couples to the electric ﬁeld-gradient (EFG) Vxx (a ¼ x,y,z). Therefore, the 75As-NMR spectrum is sensitive to a structural phase transition, as below Ts the EFG will change appreciably. Such change was indeed conﬁrmed in the parent compounds BaFe2As2 (ref. 17) and LaFeAsO (ref. 27). When a magnetic ﬁeld H0 is applied in the ab plane, the NMR resonance frequency f is expressed by 1 1 fm$m 1 ðf; ZÞ ¼ f0 þ nQ m ðZ cos 2f 1Þ ð1Þ 2 2

NATURE COMMUNICATIONS | 4:2265 | DOI: 10.1038/ncomms3265 | www.nature.com/naturecommunications

& 2013 Macmillan Publishers Limited. All rights reserved.

ARTICLE

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms3265

75As-NMR intensity (a.u.)

100

1/T1 (s–1)

10

BaFe1.95Ni0.05As2 H0 a or b H0 = 11.999 T 100 K 80 K

x = 0.05 x = 0.07 x = 0.09 x = 0.10 x = 0.12 x = 0.14

1

0.1 10

75As-NMR intensity (a.u.)

BaFe2–xNixAs2 BaFe1.93Ni0.07As2 H0 a or b H0 = 11.999 T 80 K 60 K

100

75As-NMR intensity (a.u.)

where m ¼ 3/2, 1/2 and 1/2, j is the angle between H0 and the a axis, nQ is the nuclear quadrupole resonance frequency, which is jVxx Vyy j . For a tetragonal proportional to the EFG, and Z Vzz crystal structure, Z ¼ 0. For an orthorhombic structure, however, the a axis and b axis are not identical, which results in an asymmetric EFG so that Z40. Therefore, for a twined single crystal, the ﬁeld conﬁgurations of H0|| a axis (j ¼ 0°) and H0|| b axis (j ¼ 90°) will give a different fm2m 1(j,Z), leading to a splitting of a pair of the satellite peaks into two. The above argument also applies to the case of electronic nematic phase transition such as orbital ordering, as the EFG is also sensitive to a change in the occupation of the on-site electronic orbits. As shown in Fig. 7a,b, only one pair of satellite peaks is observed at high temperature for both x ¼ 0.05 and 0.07. Below certain temperature, Ts, however, we observed a splitting of the satellite peaks. This is strong microscopic evidence for a structural transition occurring in the underdoped samples, where the NMR spectra split owing to the formation of the twinned orthorhombic domains. In fact, each satellite peak can be well reproduced by assuming two split peaks. The obtained Ts ¼ 90 K for x ¼ 0.05 and Ts ¼ 70 K for x ¼ 0.07 agrees well with the resistivity data where an upturn at Ts is observed, see Fig. 8. This feature in the spectra persists to the higher dopings x ¼ 0.10 and 0.12. For the optimal doping x ¼ 0.10, the spectrum is nearly unchanged for 40 KrTr60 K, but suddenly changes at 20 K. This indicates that a structural transition takes place below Ts ¼ B40 K for this doping composition. For x ¼ 0.12, the two satellite peaks do not change at high temperatures, but shift to the opposite direction below T ¼ 10 K. Each broadened peak at T ¼ 6 K can be well ﬁtted by a superposition of two peaks. This is the ﬁrst observation that a structural phase transition takes place below Tc. For x ¼ 0.14, however, no broadening of the spectra was found down to T ¼ 4.5 K; the spectrum shift to the same direction is due to a reduction of the Knight shift in the superconducting state. This indicates that Ts ¼ 0 around xc2 ¼ 0.14. The Ts results obtained by NMR are summarized in the phase diagram as shown in Fig. 2b. Therefore, the minimal n ¼ 1.1 of the resistivity exponent around xc2 implies quantum critical ﬂuctuations associated with the structural QCP. We hope that our work will stimulate more experimental measurements such as elastic constant, which is also sensitive to such critical ﬂuctuations28. It should be emphasized

75As-NMR intensity (a.u.)

Figure 6 | The 1/T1 for all the superconducting samples. The temperature dependence of the spin-lattice relaxation rate 1/T1 for various x of BaFe2 xNixAs2. The solid and dashed arrows indicate Tc and TN, respectively. The error bar is the s.d. in ﬁtting the nuclear magnetization recovery curve.

75As-NMR intensity (a.u.)

Temperature (K) BaFe1.90Ni0.10As2 H0 a or b H0 = 11.998 T 60 K 40 K 20 K

BaFe1.88Ni0.12As2 H0 a or b H0 = 11.998 T 60 K 15 K 6K

BaFe1.86Ni0.14As2 H0 a or b H0 = 11.998 T 60 K 4.5 K

85.5 86.0 86.5 87.0 88.0 88.5 89.0 89.5 90.0 Frequency (MHz) Figure 7 | The satellite peaks corresponding to the 21 ! 32 and 32 ! 21 transitions. (a–d) The satellite peaks with the external ﬁeld H0 applied along the a axis or b axis above and below Ts for x ¼ 0.05, 0.07, 0.10 and 0.12. The peaks split below Ts due to a change in EFG. All the spectra are ﬁtted by a single Gaussian function above Ts, but by two Gaussian functions below Ts. (e) The satellite peaks for x ¼ 0.14, which only shift to the same direction due to a reduction of the Knight shift as in Fig. 3c.

here that the exponent n ¼ 1.1 is smaller than n ¼ 4/3 expected for the ﬂuctuations dominated by q ¼ (0,0) (ref. 12). Our result suggests that the ﬂuctuation associated with xc2 is local (namely, all wave vectors contribute to the quasiparticles scattering), which would lead to an n ¼ 1 (ref. 29). Discussion The mechanism for the superconductivity in iron-pnictides has been discussed in relation to magnetic ﬂuctuations30–32 as well as structural/orbital ﬂuctuations33. In this context, it is worthwhile

NATURE COMMUNICATIONS | 4:2265 | DOI: 10.1038/ncomms3265 | www.nature.com/naturecommunications

& 2013 Macmillan Publishers Limited. All rights reserved.

5

ARTICLE

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms3265

1 BaFe1.93Ni0.05As2

BaFe1.93Ni0.07As2

0.34

0.68

–2

0.28

0 0.64

–1 Ts

0.26

TN

–4 40

0.6

TN

Ts

ab (mΩ cm)

0.3

dab /dT (μΩ cm K–1)

0.32 ab (mΩ cm)

dab/dT (μΩ cm K–1)

0

–2

60 80 100 120 Temperature (K)

40

60 80 100 Temperature (K)

Figure 8 | The enlarged part of the electrical resistivity and its derivative for the underdoped samples. (a) Enlarged part of the in-plane electrical resistivity rab (right vertical axis) and its derivative (left vertical axis) for x ¼ 0.05. (b) Data for x ¼ 0.07. The solid and dashed arrows indicate the structural phase transition temperature Ts and the antiferromagnetic transition temperature TN determined by NMR, respectively.

noting that Tc is the highest around xc1. This suggests that the superconductivity in BaFe2 xNixAs2 is more closely related to the antiferromagnetic QCP rather than the structural QCP. Also, previous results suggestive of a magnetic QCP was reported for BaFe2(As1 xPx)2 (refs 34,35), but isovalent P substitution for As does not add carriers there. In the present case, Ni directly donates electrons into the system (chemical doping), so the tuning parameter is totally different here. Thus, our work demonstrates that BaFe2 xNixAs2 is a new material that provides a unique opportunity to study the issues of quantum criticality. In particular, our result suggests that xc2 is a new type of QCP at which the exponent n cannot be explained by existing theories. Although the importance of the tetragonal-toorthorhombic structural transition, which is often associated with electronic nematicity36,37, has been pointed out in the pnictides33,38,39, the physics of a QCP associated with it is a much less-explored frontier, which deserves more investigations in the future. Methods Sample preparation and characterization. The single crystal samples of BaFe2 xNixAs2 used for the measurements were grown by the self-ﬂux method40. Here the Ni content x was determined by energy-dispersive x-ray spectroscopy. The Tc was determined by DC susceptibility measured by a superconducting quantum interference device with the applied ﬁeld 50 Oe parallel to the ab plane. The Tc is 3.5, 14, 18.5, 18.2, 16.8 and 13.1 K for x ¼ 0.05, 0.07, 0.09, 0.10, 0.12 and 0.14, respectively. The resistivity measurements. Resistivity measurements were performed in quantum design physical properties measurement system by a standard dc fourprobe method. Here we have used the same single crystals used in the NMR measurements. The electrical resistance was measured upon both warming and cooling processes in order to ensure no temperature effect from the electrodes on the samples. Both the warming and the cooling speed is 2 K min 1. Measurements of NMR spectra and T1. The NMR spectra were obtained by integrating the spin echo as a function of the RF frequency at a constant external magnetic ﬁeld H0 ¼ 11.998 T. The nucleus 75As has a nuclear spin I ¼ 3/2 and the nuclear spin Hamiltonian can be expressed as H ¼ ghI ðH0 þ Hint Þ þ

hnQ 1 3IZ2 I ðI þ 1Þ þ Z I 2þ þ I 2 6 2

ð2Þ

where g/2p ¼ 7.9219 MHz T 1 is the gyromagnetic ratio of 75As, h is Planck constant, Hint is the internal magnetic ﬁeld at the As nuclear spin site resulting from the hyperﬁne coupling to the neighbouring Fe electrons. The T1 was determined by using the saturation-recovery method and the nuclear magnetization is ﬁtted to 1 MMðð1tÞÞ ¼ 0:9 exp 6t=T1 þ 0:1 exp t=T1 , where 6

M(t) is the nuclear magnetization at time t after the saturation pulse41. The curve is ﬁtted very well and T1 is of single component. Simulation of the spectra. In order to reproduce the spectra, we assume that the distribution of the internal magnetic ﬁeld is Gaussian as, ff ½gðH0 hHint iÞ þ nnc g2 I ð f Þ ¼ exp 2Hs2

ð3Þ

where I(f) is the intensity of the spectra, Hs is the distribution of the internal magnetic ﬁeld Hint, and nc is the nuclear quadrupole resonance frequency tensor along the c axis. Then the spectrum is ﬁtted by convoluting equation 3 with a f 02 1ﬃ Gaussian broadening function pðf 0Þ ¼ An pﬃﬃﬃ exp 2s that already exists 2 2psn n pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ above TN. For n ¼ 0 (central transition), A0 ¼ 1 and 2 2 ln 2s0 is the full-width at ± half maximum (FWHM) pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ of the central peak above TN. For n ¼ 1 (satellites), A±1 ¼ 3/4 and 2 2 ln 2s 1 is the FWHM of satellite lines above TN. The red solid pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ curve in Fig. 3a is a ﬁt with Hs ¼ 0.37 T, 2 2 ln 2s0 ¼ 0.03 MHz and pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 ln 2s 1 ¼ 0.38 MHz, which was taken from the spectrum at T ¼ 100 K. The pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ red solid curve in Fig. 3b is a ﬁt with 2 2 ln 2s0 ¼ 0.04 MHz and pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 ln 2s 1 ¼ 0.5 MHz, which was taken from the spectrum at T ¼ 50 K.

References 1. Cooper, R. A. et al. Anomalous criticality in the electrical resistivity of La2 xSrxCuO4. Science 323, 603–607 (2009). 2. Mathur, N. D. et al. Magnetically mediated superconductivity in heavy fermion compounds. Nature 394, 39–43 (1998). 3. Gegenwart, P., Si, Q. & Steglich, F. Quantum criticality in heavy-fermion metals. Nat. Phys 4, 186–197 (2008). 4. Coleman, P. & Schoﬁeld, A. J. Quantum criticality. Nature 433, 226–229 (2005). 5. Kamihara, Y., Watanabe, T., Hirano, M. & Hosono, H. Iron-based layered superconductor La[O1 xFx]FeAs (x ¼ 0.05-0.12) with Tc ¼ 26 K. J. Am. Chem. Soc. 103, 3296–3297 (2008). 6. Rotter, M., Tegel, M. & Johrendt, D. Superconductivity at 38 K in the iron arsenide (Ba1 xKx)Fe2As2. Phys. Rev. Lett. 101, 107006 (2008). 7. Oka, T. et al. Antiferromagnetic spin ﬂuctuations above the dome-shaped and full-gap superconducting states of LaFeAsO1 xFx revealed by 75As-nuclear quadrupole resonance. Phys. Rev. Lett. 108, 047001 (2012). 8. Hertz, J. A. Quantum critical phenomena. Phys. Rev. B 14, 1165–1184 (1976). 9. Chakravarty, S., Halperin, B. I. & Nelson, D. R. Two-dimensional quantum Heisenberg antiferromagnet at low temperatures. Phys. Rev. B 39, 2344–2371 (1989). 10. Kasahara, S. et al. Evolution from non-Fermi- to Fermi-liquid transport via isovalent doping in BaFe2(As1 xPx)2 superconductors. Phys. Rev. B 81, 184519 (2010). 11. Moriya, T. Theory of itinerant electron magnetism. J. Mag. Mag. Mat 100, 261–271 (1991). 12. Xu, C., Muller, M. & Sachdev, S. Ising and spin orders in the iron-based superconductors. Phys. Rev. B 78, 020501 (2008).

NATURE COMMUNICATIONS | 4:2265 | DOI: 10.1038/ncomms3265 | www.nature.com/naturecommunications

& 2013 Macmillan Publishers Limited. All rights reserved.

ARTICLE

NATURE COMMUNICATIONS | DOI: 10.1038/ncomms3265

13. Li, L. J. et al. Superconductivity induced by Ni doping in BaFe2As2 single crystals. N. J. Phys 11, 025008 (2009). 14. Sefat, A. S. et al. Superconductivity at 22 K in Co-doped BaFe2As2 crystals. Phys. Rev. Lett. 101, 117004 (2008). 15. Luo, H. Q. et al. Coexistence and competition of the short-range incommensurate antiferromagnetic order with the superconducting state of BaFe2 xNixAs2. Phys. Rev. Lett 108, 247002 (2012). 16. Dioguardi, A. P. et al. Local magnetic inhomogeneities in Ba(Fe1 xNix)2As2 as seen via 75As NMR. Phys. Rev. B 82, 140411 (2010). 17. Kitagawa, K., Katayama, N., Ohgushi, K., Yoshida, M. & Takigawa, M. Commensurate itinerant antiferromagnetism in BaFe2As2: 75As-NMR studies on a self-ﬂux grown single crystal. J. Phys. Soc. Jpn 77, 114709 (2008). 18. Li, Z. et al. Microscopic coexistence of antiferromagnetic order and superconductivity in Ba0.77K0.23Fe2As2. Phys. Rev. B 86, 180501 (2012). 19. Ning, F. L. et al. Contrasting spin dynamics between underdoped and overdoped Ba(Fe1 xCox)2As2. Phys. Rev. Lett. 104, 037001 (2010). 20. Korringa, J. Nuclear magnetic relaxation and resonnance line shift in metals. Physica 16, 601–610 (1950). 21. Ikeda, H. Pseudogap and superconductivity in iron-based layered superconductor studied by ﬂuctuation-exchange approximation. J. Phys. Soc. Jpn 77, 123707 (2008). 22. Tabuchi, T. et al. Evidence for a full energy gap in the nickel pnictide superconductor LaNiAsO1 xFx from 75As nuclear quadrupole resonance. Phys. Rev. B 81, 140509 (2010). 23. Hlubina, R. & Rice, T. M. Resistivity as a function of temperature for models with hot spots on the Fermi surface. Phys. Rev. B 51, 9253–9261 (1995). 24. Fujimoto, S., Kohno, H. & Yamada, K. Temperature dependence of electrical resistivity in two-dimension Fermi systems. J. Phys. Soc. Jpn 60, 2724–2728 (1991). 25. Huang, Q. et al. Neutron-diffraction measurements of magnetic order and a structural transition in the parent BaFe2As2 compound of FeAs-based hightemperature superconductors. Phys. Rev. Lett. 101, 257003 (2008). 26. Pratt, D. K. et al. Coexistence of competing antiferromagnetic and superconducting phases in the underdoped Ba(Fe0.953Co0.047)2As2 compound using X-ray and neutron scattering techniques. Phys. Rev. Lett. 103, 087001 (2009). 27. Fu, M. et al. NMR search for the spin nematic state in LaFeAsO single crystal. Phys. Rev. Lett. 109, 247001 (2012). 28. Yoshizawa, H. et al. Structural quantum criticality and superconductivity in iron-based superconductor Ba(Fe1 xCox)2As2. J. Phys. Soc. Jpn 81, 024604 (2012). 29. Watanabe, S. & Miyake, K. Quantum valence criticality as an origin of unconventional critical phenomena. Phys. Rev. Lett. 105, 186403 (2010). 30. Mazin, I. I., Singh, D. J., Johannes, M. D. & Du, M. H. Unconventional signreversing superconductivity in LaFeAsO1 xFx. Phys. Rev. Lett. 101, 057003 (2008). 31. Kuroki, K. et al. Unconventional pairing originating from the disconnected Fermi surfaces of superconducting LaFeAsO1 xFx. Phys. Rev. Lett. 101, 087004 (2008). 32. Graser, S. et al. Spin ﬂuctuations and superconductivity in a three-dimensional tight-binding model for BaFe2As2. Phys. Rev. B 81, 214503 (2010).

33. Kontani, H. & Onari, S. Orbital-ﬂuctuation-mediated superconductivity in iron pnictides: analysis of the ﬁve-orbital Hubbard-Holstein model. Phys. Rev. Lett. 104, 157001 (2010). 34. Nakai, Y. et al. Unconventional superconductivity and antiferromagnetic quantum critical behavior in the isovalent-doped BaFe2(As1 xPx)2. Phys. Rev. Lett. 105, 107003 (2010). 35. Hashimoto, K. et al. A sharp peak of the zero-temperature penetration depth at optimal composition in BaFe2(As1 xPx)2. Science 336, 1554–1557 (2012). 36. Chu, J.-H. et al. In-plane resistivity anisotropy in an underdoped iron arsenide superconductor. Science 329, 824–826 (2010). 37. Yi, M. et al. Symmetry breaking orbital anisotropy on detwinned Ba(Fe1 xCox)2As2 above the spin density wave transition. Proc. Natl Acad. Sci. USA 108, 6878–6883 (2011). 38. Fernandes, R. M., Chubukov, A. V., Knolle, J., Eremin, I. & Schmalian, J. Preemptive nematic order, pseudogap, and orbital order in the iron pnictides. Phys. Rev. B 85, 024534 (2012). 39. Yanagi, Y., Yamakawa, Y., Adachi, N. & Ono, Y. Cooperative effects of Coulomb and electron-phonon interactions in the two-dimensional 16-band d-p model for iron-based superconductors. Phys. Rev. B 82, 064518 (2010). 40. Sun, D. L., Liu, Y., Park, J. T. & Lin, C. T. Growth of large single crystals of BaFe1.87Co0.13As2 using a nucleation pole. Supercond. Sci. Technol. 22, 105006 (2009). 41. Narath, A. Nuclear spin-lattice relaxation in hexagonal transition metals: titanium. Phys. Rev. 162, 320–332 (1967).

Acknowledgements We thank Q. Si, K. Miyake, K. Kuroki, T. Takimoto, R. Fernandes, T. Xiang, Y. Yanase and S. Fujimoto for helpful discussion. This work was partially supported by National Basic Research Program of China (973 Program), Nos. 2011CBA00100 and 2011CBA00109, and by CAS.

Author contributions The single crystals were grown by D.L.S. and C.T.L. The NMR measurements were performed by R.Z., Z.L., J.Y. and G.-q.Z. The electrical resistivity was measured by R.Z., Z.L. and J.Y. G.-q.Z. coordinated the whole work and wrote the manuscript, which was supplemented by R.Z. All authors have discussed the results and the interpretation.

Additional information Supplementary Information accompanies this paper at http://www.nature.com/ naturecommunications Competing ﬁnancial interests: The authors declare no competing ﬁnancial interests. Reprints and permission information is available online at http://npg.nature.com/ reprintsandpermissions/ How to cite this article: Zhou, R. et al. Quantum criticality in electron-doped BaFe2 xNixAs2. Nat. Commun. 4:2265 doi: 10.1038/ncomms3265 (2013).

NATURE COMMUNICATIONS | 4:2265 | DOI: 10.1038/ncomms3265 | www.nature.com/naturecommunications

& 2013 Macmillan Publishers Limited. All rights reserved.

7